Designation: D 3134 – 97Standard Practice for Establishing Color and Gloss Tolerances1 This standard is issued under the ﬁxed designation D 3134; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript epsilon (e) indicates an editorial change since the last revision or reapproval. INTRODUCTION Permissible color and gloss deviations from a standard are generally dependent upon the color discrimination of the observer, on the lighting and surround in which the material is viewed, and on special considerations related to the design, manufacture, and practical usage of the colored material or object. The tolerances, therefore, may be inﬂuenced by economic, technical, psychological, and practical requirements. In many circumstances, acceptability of color and gloss deviations from a standard may differ appreciably from the perceptibility of deviations such as on-tone fading preferences, large tolerances for luminance variation, nongreen bias, or nonyellow bias. With proper allowances, perceptibility data can be used as an aid to develop permissible tolerances. Finally, the sum of all these considerations should result in a speciﬁcation acceptable to both buyer and seller. 1. Scope 1.1 This practice describes a procedure for establishing tolerances and evaluating the color and gloss of specimens with respect to speciﬁed standards. This practice is appropriate for nonﬂuorescent opaque specimens. 1.2 This practice does not indicate the extent of tolerances, but gives guidance on how they can be set. For product speciﬁcation, the tolerances between specimens and the speciﬁed standard should be agreed upon between the purchaser and the seller. 1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. 2. Referenced Documents 2.1 ASTM Standards: D 523 Test Method for Specular Gloss2 D 1535 Practice for Specifying Color by the Munsell System2 D 1729 Practice for Visual Evaluation of Color Differences of Opaque Materials2 D 2244 Test Method for Calculation of Color Differences from Instrumentally Measured Color Coordinates2 D 3964 Practice for the Selection of Coating Specimens for Appearance Measurement2 1 This practice is under the jurisdiction of ASTM Committee E12.11 on Visual Methods and is the direct responsibility of Subcommittee E-12 on Appearance of Materials. Current edition approved Feb. 10, 1997. Published September 1997. Originally published as D 3134 – 72 T. Last previous edition D 3134 – 89. 2 Annual Book of ASTM Standards, Vol 06.01. D 4449 Test Method for Visual Evaluation of Gloss Differences Between Surfaces of Similar Appearance2 D 5531 Guide for the Preparation, Maintenance, and Distribution of Physical Product Standards for Color and Geometric Appearance of Coatings2 E 284 Terminology of Appearance2 E 308 Practice for Computing the Colors of Objects by Using the CIE System2 E 312 Practice for Description and Selection of Conditions for Photographing Specimens2 E 805 Practice for Identiﬁcation of Instrumental Methods of Color and Color-Difference Measurement of Materials2 E 1164 Practice for Obtaining Spectrophotometric Data for Object-Color Evaluation2 E 1331 Test Method for Reﬂectance Factor and Color by Spectrophotometry Using Hemispherical Geometry2 E 1345 Practice for Reducing the Effect of Variability of Color Measurements by the Use of Multiple Measurements2 E 1349 Test Method for Reﬂectance Factor and Color by Spectrophotometry Using Bidirectional Geometry2 E 1360 Practice for Specifying Color Using the Optical Society of America Uniform Color Scales System2 E 1499 Guide to the Selection, Evaluation, and Training of Observers2 E 1541 Practice for Specifying and Matching Color Using the Colorcurve System2 E 1708 Practice for Electronic Interchange of Color and Appearance Data2 2.2 CIE Publication: Copyright © ASTM, 100 Barr Harbor Drive, West Conshohocken, PA 19428-2959, United States. 1 2. 7 Pond St.1.3 Measure the gloss in accordance with Test Method D 523. whether examined visually or instrumentally. CIE 1976 hue-angle. or both. 7. Correspondingly. 7.1 Select a standard in accordance with Practice D 3964 that is preferably the same type of material as the specimens to be evaluated for color or gloss. In the case of visual evaluation of the effect of color and gloss. gloss speciﬁcations are centered around an exact position on the gloss scale. or E 1541. Signiﬁcance and Use 5.1 The exact method of preparation of the specimen shall be agreed upon between the purchaser and the seller. Thomas Lemons. TLA Lighting Consultants. The CIE terminology appropriate to this usage is CIE 1976 lightness.D 3134 No. While this color metric (CIELAB) is convenient for expressing color differences. (If the standard is textured.) The variability of the measurements due to texture may be reduced by following the recommendations outlined in Practice E 1345. Measure the color in accordance with Practices E 1164 and E 805. Prepare. uniform in color. and uniform in texture.1.1 Selection and Speciﬁcation of Color and Gloss Standard: 7.1. note the texture orientation during measurement. Selection of the magnitude and direction of color tolerances shall be based on careful consideration of all applicable factors. E 1360. The CIELAB 1976 hue-angle and chroma are illustrated in Fig. MA 01970–4819.1.2 Gloss differences can affect instrumental measurement of color differences. it should be recognized that signiﬁcant differences in surface texture between standard and test specimens signiﬁcantly affect both color and gloss. Do this even if the standard is textured. 15. 4. and costs of controlling the magnitude and direction of color difference. it is necessary to specify tolerances that are acceptable to both the buyer and the seller. 7.1.1 In order to obtain a permanent record. in the permanent material. Preferred sizes of specimens for visual evaluation are given in Practice D 1729. 7. While Practice D 3134 does not deal with texture tolerances or speciﬁcations. Standards should have the same spectral characteristics as the manufactured product. 6. 5. However.2 and Practice E 308. For example. tolerances may be selected on the basis of perceptibility of the magnitude of color difference.3 When color difference formulae are used in practice.2. See Test Method D 2244 and Method E 308. 7. The CIE 1976 L*a*b* (CIELAB) approximately uniform color space and color difference equations have been recommended for use by the International Commission on Illumination (CIE).1 This practice consists of recommendations for the selection of a standard. be aware that changes in gloss values may have an effect upon color measurements. Specimens 6. 1.2.2 Colorimetry 2nd ed.1 Deﬁnitions—For deﬁnitions of terms related to this practice see Terminology E 284.1 Color speciﬁcations are centered around exact positions in color space.. Large gloss differences between visually identical colors can cause their color measurements to exhibit larger color differences than in fact exist. exercise care to limit the specimens to those that have quite similar gloss values. Terminology 3. hab. 2 3 Available from the USNC-CIE Publications Office. This is usually accomplished by use of the same colorant composition.4 Employ photography for permanently recording the appearance of the surface texture (see Practice E 312). Refer to Test Methods D 2244 and Practice E 308 for equations and deﬁnitions. When using historical data to establish color tolerances.2 Selection and Speciﬁcation of Color Tolerances: 7. This practice details the procedure for accomplishing this goal. It is also desirable to express color speciﬁcations in terms of such correlates. or evaluate it in accordance with Test Method D 4449. and CIE 1976 chroma. and perceived chroma (saturation). . 7. Summary of Practice 4. Report the color as described in Practice E 308. in terms of correlates of lightness. rejection of or closer limits on certain directions of color difference. 7. Recommendations on color scales appear in CIE Publication No.1. the necessary physical measurements to assess the permanence of the standard to reproduce it when needed. plane. Salem. 7. hue. The specimens should be relatively permanent. and to establish tolerances. secondary standards in accordance with Guide D 5531 that are representative of the desired color and gloss.2.1. and capable of being cleaned. 15. for the highest precision in instrumental measurements the specimens should be opaque. Procedure 7. The standard should have the same texture as the manufactured product.1. it must be understood that a given calculated color difference in one region of color space may not represent the same visual difference in other regions of color space. 4.1. % Mr. use Practice E 805 and either Test Method E 1331 or Test Method E 1349 to correctly identify the instrumental measurement method.1 The purchaser and the seller shall agree on color tolerances with respect to a previously selected standard and on the color scales in which they are expressed. the speciﬁc size being governed by the use of the specimens.1.3 3. C*ab. When establishing gloss tolerances.2 Visual Color Assessment—Use Guide E 1499 to select an observer for the assessment. it is often desirable to identify the components of color difference. Because it is difficult to achieve these exact positions repeatedly. 7. Assess and specify the color in terms of a color system described in Practices D 1535. differences can be minimized by strict adherence to recommended illuminating and viewing geometry (see Practice D 1729).1 Express color differences between the specimen and the standard in terms of a set of three independent parameters. incorporated in the same manner into the same material.2 Recommendations are given for the determination of the conformance of a specimen to preestablished color and gloss tolerances by instrumental or visual means. in sufficient quantity. 5. 7. 3(b) show plots of specimens rated by multiple observers with respect to how well they match a standard.2. a line perpendicular to the constant-hue line and passing through the standard color is a line of constant chroma (or saturation) and becomes the minor axis of the ellipse..0 point and the tolerance ellipses deﬁne permissible differences from it. 2 (a) and Fig. This line of constant hue becomes the major axis. along with ﬁgures deﬁning the tolerances. Fig.2. 0) through the standard color on the a*b* plot. rejected. with a* data also shown. (2) plot them. Db*) as shown .) FIG.2.5. and Saltzman. To illustrate the principle recommended: (1) rate a number of specimens for acceptability. 2(a) shows chromaticity tolerances in a* and b*.2.5. Fig. 7. Jr. (Reprinted by permission of John Wiley & Sons. F... NY.4 The CIELAB opponent-color red-green coordinate a*. W.2. or considered borderline). a*.5.D 3134 7. b*) into color difference values (DL*.2. Da*.3 To determine lightness tolerances it is necessary to plot the data for the same colors on a graph showing L* along with either a* and b*. 1981. Fig. Sample Point 2 has a larger value of hab than Point 1 and therefore is yellower in hue. 2(a). Fig. Principles of Color Technology. 2nd ed. 3(b) are changed from absolute values (L*. 2(a) and Fig. 3(b) shows lightness tolerances in L*..2 In such cases it is customary to plot the hue angle of the standard by drawing a line from the origin (0. the copyright owner. 7. and (3) prepare to draw the tolerance ﬁgure dictated by the data. Point 2 also has a smaller value of Cab* than Point 1 and is therefore lower in chroma or duller. John Wiley and Sons. NOTE 2—Original source is Billmeyer. 3(b). and draw a tolerance ellipse as in Fig. Chroma is measured as the length of the line from the neutral point (a* 5 b* 5 0) to the sample point. if the data plot indicates the ellipse should be symmetrical around the standard color. 1 CIE 1976 L* a * b* (CIELAB) Hue Angle and Chroma (a) Chromaticity Tolerances NOTE 1—The standard color is at the 0. and the yellow-blue coordinate b* are deﬁned in Test Method D 2244 and Practice E 308. 2 Plots of Instrumental Results on Color Specimens Along With Their Visual Acceptability Ratings 3 . FIG. 7.5 Graphical Interpretation of Historical Data: 7. These lines assist in drawing the tolerance ellipse. NOTE 1—Hue angle is measured in degrees starting with hab 5 0 in the + a* (red) direction and increasing counterclockwise.1 Color tolerances can be determined from a graphical interpretation of historical data (batches accepted. New York. The choice between a* and b* is dictated by which of these attributes cover the greater range.4 The scales on Fig. M. Similarly. the graphical representation is a regular geometric ﬁgure that can be represented mathematically.2. the visual gloss tolerance will be symmetrical around the nominal value of the standard. Frequently when it is necessary to set color tolerances.0 point and the tolerance ellipses deﬁne permissible differences from it. Fig. and the standard color may be far from its center. The nongreen and nonyellow biases mentioned in the introduction are but two of these. It will . inspection should be under speciﬁed light sources following the recommendations in Practice D 1729. 2(a) and Fig. color tolerances will not be symmetrically located in all directions about the standard color in any color space. 7. Such representation may involve some sacriﬁce in accuracy of the tolerance speciﬁcation and should be used with care.9 When tolerance standards are prepared to illustrate the color in the hue.8 Finally. 7. lightness. and saturation or chroma attributes of color space and to allow visual interpretation of the conformity of color.7 In general. 3 Plots of Instrumental Results on Color Specimens Along With Their Visual Acceptability Ratings 7. with a* data also shown. there are many deviations from the regular geometric ﬁgures described in 7. 2(a) shows chromaticity tolerances in a* and b*. its major axis may deviate from the direction of constant hue. and two adjacent hue limits.2.2. the 4 tolerance ﬁgure may not be regular.D 3134 (b) Lightness Tolerances NOTE 1—The standard color is at the 0. to ensure that they appropriately address the color quality control requirement. 3(b).2. in some instances the asymmetry may be small enough that the color tolerances may be represented by a single. overall color difference (DE) that represents the radius of a sphere about the standard in color space. perhaps it will be an ovoid instead of an ellipse. once set. (see Fig.2. It is therefore necessary to monitor tolerances.2 With few exceptions.6 When tolerances for each color attribute (hue. FIG. 7. 7.3. It is also common to represent color tolerances by a set of six points: light and dark limits.6 and depicted in Fig. and saturation or chroma) are symmetrical in the plus and minus directions. 3(b)). Fig.3. as by the equation for an ellipse or an ellipsoid. low and high saturation limits. 2(a) and Fig. lightness. However.1 The gloss tolerances around the gloss of the standard may be expressed in gloss units (See Test Method D 523) or as a percent. the amount of historical accept-reject data will be too modest for this purpose. 3(b) shows lightness tolerances in L*. For example.3 Selection and Speciﬁcation of Gloss Tolerances: 7. Gonioapparent coatings or materials require special methodologies for viewing and measurement. 7. and should not be considered as recommendations. lightness. DG High Low +4 −6 +8 −12 +12 −18 This example is for illustration purposes only. and O’Donnell.4.5 units in L* as a tight tolerance.6. 7. 7. Asymmetrical color tolerances around a standard color represent the usual case.4 If tolerance standards are prepared to show visually the upper and lower limits for gloss. if a lightness tolerance of 62. These are 5 examples only. The expected result is that visually acceptable specimens will be grouped about the standard (plotted as Da* 5 Db* 5 0). Compare the specimen with the visual standards under the viewing conditions described in Practice D 1729.4.1 Tolerances should be set by agreement between the purchaser and the seller. 7. However.0 (DL* 5 62.D 3134 be necessary to determine experimentally the instrumental readings that correspond to the required visual differences. If both ﬁgures can be approximated by circles of similar radii.4.4 Liberal tolerances are used.4. equal instrumental gloss values do not necessarily represent equal visual gloss differences.3 When the gloss desired is at or near the maximum or minimum gloss attainable. and lightness tolerances to be less tight. 7. 7. The LV should be experimentally determined so that LV/3 represents the least discernible gloss difference. W.1 The usual requirement is that the gloss tolerances above and below the gloss of the standard be visually equal. it is customary to specify a single gloss reading and the direction in which the data may depart from it. Tight tolerances are used for ﬁnishes on consumer products. 7. and saturation or chroma. they should preferably be of the same color and material as the standard. whichever results vary more. it is a useful basis for setting tighter or more liberal tolerances in the original color region. known buyer requirements. and porcelain insulators on poles.4. (A 10 % increase in each attribute equals a 33 % increase in volume). then measuring the specimens and standard and plotting the values on a CIELAB Da*.5 and 7.. X. automobiles and major appliances. not recommendations. The values 4 Billmeyer.0 In this example the A tolerance is the tightest.4.4 A lightness tolerance DL* must also be established. it can be stated that the usual tolerance speciﬁcation requires hue tolerances to be relatively tighter. Tentative tolerances can be based on the guidelines given in 7. D. so that a small incremental increase in each attribute results in a substantial increase in total tolerance volume.6. around a speciﬁc color.5.3 Tolerances are preferably set experimentally by classifying specimens visually against a visual standard.4. because there are important differences between equally perceptible and equally acceptable differences. it is expected that a ﬁgure can be drawn enclosing the data range for acceptable specimens. exact color matches are seldom seen. Examples are color-coded electronic parts and wires. one might specify “80 units minimum. DE 1. p.4. 7.6.3 Keep in mind that the total color difference is a combination of those allowed for each of the three attributes. These numbers are intended only as examples.2 The most frequently encountered industrial tolerances provide for different limits for the visual color attributes of hue. the seller shall set tolerances unilaterally.3. 1987. Thus. Tolerances shall be speciﬁed in the same Test Method D 523 gloss scale as used to specify the gloss of the standard. for a very high gloss requirement. at times the purchaser is either unknown (as in the case of consumer products) or unequipped to determine tolerances based on instrumental measurement. Again. based upon such considerations as the economics of the production process.’’ Similarly.4. one might then choose 61.4. typically. in a variety of glosses. with saturation or chroma tolerances between these. 7.1 Symmetrical color tolerances around a standard color can be speciﬁed in terms of the overall color difference (DE) in CIELAB units (see Test Method D 2244 and Practice E 308).5. with a corresponding increase in cost. .5 Color Tolerances: 7. can be used. the material used is difficult to color accurately or the products exhibit large variations in other appearance attributes (texture or gloss) which tend to mask color differences or are seen only from a distance. while the C tolerance is the most liberal. it may be appropriate to specify a maximum total color difference DE as the tolerance.4. Therefore. Conversely. In such cases. Tolerance Designation A B C CIELAB Color Difference.6 Gloss Tolerances: 7. 7.4. F. one must realize that some tolerance is necessary.0 2. A rough approximation is the lightness difference DL* for colors that match the standard in hue and saturation.5 units as a more liberal tolerance.4.5 Only specimens that fall within the deﬁned limits are acceptable... F. However. Vol 12. 7.0) units was selected as intermediate.4 Tolerance Classiﬁcation: 7. 7. Db* constant-lightness (L*) plane. and similar products.4. when the product is very small. more accurate to plot differences DL* and either Da* or Db*. Jr. colored masonry. 315.2 It has been found useful to specify tolerances around a standard gloss in terms of a limiting value (LV). or 62. commercially available gloss scales showing a large number of samples of the same color. Color Research and Application. as shown in the following example. 7. A modest reduction in tolerance can cause an important increase in difficulty of matching. It is however. so that a line enclosing them forms a ﬁgure on the Da*Db* plane. Variations from this exist. it is necessary to specify the high and low gloss tolerances separately.0 3. For example. The permissible specular gloss tolerances (DG) can then be as follows: Tolerance Designation LV/3 2LV/3 LV Gloss Tolerance. 7.’’ with the measurement geometry being indicated in each case.5. However.3.5. research4 has shown that even for small gloss differences. such as.5.4.2 While a CIELAB color difference applicable to one region of color space may not be transferable to other regions of color space. for a very low gloss the speciﬁcation might read “3 units maximum. While it is beyond the scope of this practice to discuss these differentials in detail. are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised.3 For visual color difference evaluation.1 Because the quality and quantity of illumination is important in visual color difference evaluations. or through the ASTM website (http://www. colorcurve system. 10. Precision and Bias 11. no basis for deﬁning bias.16 Time and date of the gloss measurement. which you may attend. 9. 12.3 Report the measurement conditions (specular included or excluded) and the CIE color-matching functions and illuminant for which the data are computed.2 Data may be reported in electronic format. 11. D 2244. PA 19428-2959.1 The precision of the instrumental measurements is stated in Practice E 1164 and Test Methods D 523.1.9 Gloss measurements of standard and specimens. reﬂection haze. 100 Barr Harbor Drive. Report 10. 8. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone). the closer these specimens are to each other. use Test Method D 523. 10. gloss. Precision is also related to the amount of gloss and color difference portrayed by the physical specimens representing standards and tolerances.8 Designation of calibration standard for color measurement. Munsell system. Practice D 1729 may be applied.12 Identity of observer or instrument operator by name or code designation. Evaluation of Compliance with Tolerance Limits 9. and E 1349.1.1 Evaluate compliance either instrumentally or visually. 10. E 1331. 10. or [email protected]
Light Sources 8.org).7 Time and date of last color instrument calibration. For both color and gloss measurements. PA 19428.D 3134 vary with geometry and with their position on the gloss scale. 10.17 Time and date of last calibration of gloss meter. 10.1.6 Time and date of color measurement.1. either reapproved or withdrawn. 11. 9.18 Designation of calibration standard for gloss measurement.10 Observed texture differences between standard and specimens. For visual gloss difference. 10. glossmeter. 11.1. 10. West Conshohocken. Optical Society of America Uniform Color Scales system. Your comments will receive careful consideration at a meeting of the responsible technical committee. the illuminating and viewing conditions used. gloss tolerances. See Practice D 1729.1. such as distinctness of reﬂected image. model number. color difference. 10. hence. 10.11 If visual tolerance standards are employed. West Conshohocken. Practices E 1164 and E 308 may be applied where spectrophotometers are used. 10. and 10. are not covered by this simple classiﬁcation scheme. 10. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards. see Practice E 1708. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM Headquarters.13 Identity of color and gloss measuring instruments.1 Designation of standards and specimens.1. it is important that related measurements be made in consecutive order by the same operator and on the same instrument for maximum precision. use Method D 4449.5 Color instrument manufacturer.4 For instrumental gloss difference. the higher the precision. and texture. 9. Keywords 12.astm.4 Observed direction and magnitude of color departure from the color standard. color tolerances.1.3 Bias—There is no deﬁnition of an agreed upon reference standard. United States. report the following information: 10. Users of this standard are expressly advised that determination of the validity of any such patent rights. spectrophotometer The American Society for Testing and Materials takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard.15 Gloss instrument manufacturer model number and serial number.2 Color measurement values for the standards and specimens. 610-832-9555 (fax). and serial number. 10.1 When a report of evaluation of conformance is required.1. 9. 10.1.2 For instrumental measurement and calculation of color. 7. exercise control of the light source.14 Identity of color space and color difference formula used. 10.1.1.6.2 Much of the precision attainable in visual evaluation depends upon the skill and experience of the observer. Procedures for measuring and calculating color differences may be found in Test Method D 2244.1.1.1. This standard is copyrighted by ASTM. 10. 100 Barr Harbor Drive.1.1.3 Other important aspects of gloss. 10. and the risk of infringement of such rights.1 color. 6 . 10.org (e-mail).1.4.